Efficient Organic/Inorganic Hybrid Solar Cell Integrating Polymer Nanowires and Inorganic Nanotetrapods
© The Author(s). 2017
Received: 14 October 2016
Accepted: 14 December 2016
Published: 5 January 2017
Constructing a highly efficient bulk-heterojunction is of critical importance to the hybrid organic/inorganic solar cells. Here in this work, we introduce a novel hybrid architecture containing P3HT nanowire and CdSe nanotetrapod as bicontinuous charge channels for holes and electrons, respectively. Compared to the traditionally applied P3HT molecules, the well crystallized P3HT nanowires qualify an enhanced light absorption at the long wavelength as well as strengthened charge carrier transport in the hybrid active layer. Accordingly, based on efficient dissociation of photogenerated excitons, the interpercolation of these two nano-building blocks allows a photovoltaic conversion efficiency of 1.7% in the hybrid solar cell, up to 42% enhancement compared to the reference solar cell with traditional P3HT molecules as electron donor. Our work provides a promising hybrid structure for efficient organic/inorganic bulk-heterojunction solar cells.
KeywordsNanowire Nanotetrapod Hybrid Solar cells
Combining the potential advantage of organic semiconductor and inorganic nanocrystals, organic/inorganic hybrid bulk-heterojunction solar cell (HBSCs), one of the third generation thin-film solar cells, has attracted intense research efforts due to its unique advantage such as lightweight, low cost, good flexibility with large area, and easily tuned energy level alignment and so on. Based on extensive research efforts, the photovoltaic performance of HBSCs has been greatly improved. A power conversion of 5.5% was obtained in a hybrid containing PbSxSe1-x nanocrystals and a low-bandgap polymer .
Compared to the traditional inorganic photovoltaic semiconductors, the hybrid composites in the HBSCs have relatively low charge mobility due to the disordered orientation of organic semiconductor molecules as well as discontinuously dispersed inorganic nanocrystals [2–4], confining further improvement of photovoltaic performance of HBSCs. Regarding this problem, many efforts were taken to optimize the charge transport efficiency in the HBSCs, such as annealing of the as-prepared hybrid films , modification on structure of molecule chains [6–9], and solvent treatment [10, 11]. Most of the process aimed at enhancing orientation of molecule chains or crystallization of polymer matrix so that to increase the charge motility. Likewise, direct self-assembly of polymer molecules to form organic nanowires (NWs) (such as poly(3-hexylthiophene (P3HT))) was also proved to be helpful in achieving an enhanced charge transport as well as highly efficient organic hybrid solar cells [12, 13].
Meanwhile, to obtain an optimized phase separation in the organic/inorganic hybrids, the inorganic electron acceptor was usually prepared with good monodispersion, at the cost of high charge mobility in the bulk materials. Thus, modulation on nanoparticels’ morphology was extensively investigated to increase electron transport and collection in the HBSCs, such as nanorods and nanotubes [14–16], orientated nanoarrays [17, 18] and core-shell-shaped nanocrystals [19–21], and so on. Monodispersed nanotetrapod (NT) was also a promising candidate because of its superiority in transporting electrons through an extended charge path with three-dimensional continuity [21–23].
Thus to HBSCs, the active layer with simultaneously efficient transportation of holes and electrons is of great importance. Although organic nanowires and inorganic nanotetrapods are attractive in charge transport, there is no reported work on the HBSCs simultaneously containing these two structures. Here in this work, we have fabricated this novel organic/inorganic HBSC composed of the above two efficient nano-building blocks: P3HT NWs and CdSe NTs as donor and acceptor, respectively. The active layer enables an efficient charge transport and collection through bicontinuous pathways for holes and electrons, which is highly favored by efficient HBSCs.
Synthesis of P3HT Nanowires, CdSe Nanotetrapods, and their Hybrid
The P3HT NWs were synthesized through a self-assembly method. Typically, P3HT polymer (Sigma-Aldrich, regioregular, average Mn 54,000–75,000) was dissolved in dichlorobenzene (DCB) and heated at 80–90 °C until a clear solution was obtained. Then, the solution was filtered through a 0.45-μm filter and allowed to be slowly cooled to 5–10 °C in a day without any agitation. The solution was kept at this temperature until a purple gel was obtained, indicating the formation of P3HT NWs. This sample was kept at low temperature before it was diluted with DCB for use.
CdSe NTs were synthesized according to the procedure in a literature . Briefly, CdO (1 mmol), oleic acid (OA, 6 mmol), and 20 ml octadecene (ODE) were pumped at 140 °C under N2 flow for 30 min. After that, the temperature was raised to 260 °C at which a TOP-Se-CTAB (TOP: tri-n-octylphosphine, CTAB: Hexadecyl trimethyl ammonium Bromide) solution (containing 1 ml TOP, 0.5 mmol Se, 0.05 mmol CTAB, and 3 ml toluene) was injected quickly. The reaction was allowed and persisted for 5 min to grow the CdSe NTs. After the solution was cooled to room temperature, 10 ml acetone was injected and the red precipitation was collected by centrifugation at 4500 rpm. The obtained CdSe NTs were finally dissolved in DCB with desired concentration. The P3HT NWs:CdSe NTs hybrid solution was prepared by blending P3HT NWs and CdSe NTs DCB solution with different mass ratio and then stirring for at least 6 h. Reference sample was prepared by directly blending the traditionally dissolved P3HT molecules and CdSe NTs in DCB. All the hybrid solutions were filtered through a 0.45-μm filter before use.
Fabrication of HBSCs
Patterned ITO-coated glass substrates were cleaned sequentially with soap water, deionized water, acetone, and isopropanol under ultrasonication for 20 min. Substrates were then dried under N2 flow after which a compact TiO2 layer was deposited on top by spin-coating a titanium-acetylacetone precursor and then sintering at 450 °C for 90 min. The ITO/TiO2 substrates were transferred into a N2-filled glovebox where the fully mixed P3HT:CdSe NTs or P3HT NWs:CdSe NTs DCB solution was spin-coated. The freshly prepared hybrid films underwent solvent treatment with 1,2-ethanedithiol (EDT):methanol (10% by volume) before annealing at 150 °C for 10 min. With regard to P3HT NWs:CdSe NTs samples, keeping them in vacuum (with pressure lower than 10-2 Pa) for 12 h was required prior to heat treatment. The fabrication of hybrid solar cells was finished by evaporation of 3 nm MoO3 followed by 100 nm Ag on top. A shadow mask was used to define six separated devices each with a diameter of 2 mm.
The morphology of synthesized P3HT NWs and CdSe NTs was confirmed by high-resolution transmission electron microscope (HR-TEM, JEM-2100) at an acceleration voltage of 200 kV. The crystal structure was researched by X-ray diffraction (XRD) on a Rigaku D/max-gA X-ray diffractometer with Cu Kα radiation. Light absorption measurements were carried out on Varian Cary-5000 model Ultraviolet-visible infrared spectrophotometer. Photoluminescence (PL) spectra were collected on HORIBA Jobin Yvon Fluorlog-3 system, with exciting wavelength of 360 nm. Time-resolved photoluminescence (TRPL) spectroscopy measurements (FLSP920 lifetime spectrometers, Edinburgh Instruments, EI) were conducted using a pulse laser (380 nm) with a pulse width of 70 ps for excitation. The current-voltage characterizations were carried out using a Keithley 2440 source meter and Newport 94043A solar simulator (AM 1.5 illumination). For the surface photovoltage (SPV) spectra measurements, the samples were excited with a laser radiation pulse (wavelength of 355 nm and pulse width of 5 ns) from a third-harmonic Nd:YAG laser (Polaris II, New Wave Research, Inc.)
Results and Discussion
To investigate the exciton-splitting property in the hybrid containing the two nano-building blocks, we carried out photoluminescence characterization and the results are shown in Fig. 2c. The PL spectra for P3HT NWs exhibits two distinct emission peaks at 660 and 700 nm, corresponding to the two excitation absorption at 520 and 560 nm (Fig. 2b), respectively. It is found that a hybrid containing 80 wt% CdSe NTs could intensively quench the PL intensity of P3HT NWs, especially the main emission at 700 nm. This is interestingly the same with that of the organic polymer-grafted nanoparticles reported in ref . The static PL result indicates that the photon-generated excitons could be efficiently dissociated through diffusing in the crystallized P3HT NWs and thereafter splitting at the hybrid interface. To give additional information on the charge transfer dynamics, time-resolved photoluminescence measurement was carried out as shown in Fig. 2d. The PL lifetime analyzed by biexponential decay kinetics is 454 ps for solid state P3HT NWs, while it is 345 ps for the P3HT NWs:CdSe NTs hybrids. The PL decay of the hybrid nanostructures is much faster than that of the homopolymer, demonstrating a rapid charge transfer from P3HT NWs to CdSe NTs before radiated recombination.
Figure 3d shows the I-V characteristic of the hybrid solar cell with P3HT NWs as electron donor. For comparison, the solar cell adopting traditional P3HT molecules as donor was also fabricated and optimized as reference (named P3HT:CdSe NTs); its photovoltaic performance was also given in Fig. 3d. Under AM 1.5 illumination, the reference solar cell with traditional P3HT molecules donor generates a short current density (Jsc) of 4.5 mA/cm2, open circuit voltage (Voc) of 0.58 V, fill factor (FF) of 45.9% and conversion efficiency (Eff) of 1.2%. In comparison, hybrid solar cell incorporating P3HT NWs donor generates much better photovoltaic performance than the P3HT:CdSe NTs device, with Jsc, Voc, FF, and Eff values of 6.0 mA/cm2, 0.57 V, 49.7 and 1.7%, respectively. It should be noted that the above optimized I-V performance was obtained at an active layer thickness of 150 nm for the P3HT NWs:CdSe NTs device and 120 nm for the reference. Too thick absorber layer always decreases the performance due to much enlarged series resistance. As the P3HT NWs:CdSe NTs device performs better at a relatively thick active layer, the light absorption and charge transport ability in this bicontinuous P3HT NWs:CdSe NTs hybrid is probably higher than that in the P3HT:CdSe NTs. This also could be reflected from the observation that the performance improvement is mainly benefited from the greatly enlarged Jsc and FF values those are speculated to be closely correlated with light absorption and charge carriers transport properties of the devices [31, 32]. For further comparison, external quantum efficiency (EQE) was measured and the results are shown in Fig. 3e. EQE enhancement is observed at the wavelength from 550 to 650 nm and wavelength below 400 nm. As indicated in Fig. 2b, compared to P3HT molecules, the highly crystallized P3HT NWs have much stronger absorption at the long wavelength from 550 to 650 nm, which could partly explain the EQE enhancement at this region and the increased Jsc of the solar cell.
In conclusion, we have fabricated organic/inorganic hybrid bulk-heterojunction solar cells integrating two efficient nano-building blocks: P3HT NWs as the electron donor and CdSe NTs as the acceptor. Broad light absorption and efficient charge transport properties were retained in this novel hybrid system. More importantly, efficient charge collection and extraction were readily acquired because of the bicontinuous charge channels in the hybrids containing these two nano-building blocks. Thus compared to the traditional P3HT:CdSe NTs hybrid, an averaged enhancement of 42% in photovoltaic performance was achieved for the solar cells adopting P3HT NWs:CdSe NTs hybrid. Our work provides a novel hybrid architecture for efficient bulk-heterojunction optoelectronic devices.
This work is supported by the National Natural Science Foundation of China (Grant no. 61306019) and the National Basic Research Program of China (Grant no. 2014CB643503). This work is also supported by the Natural Science Foundation of Henan Provincial Education Department (Grant no. 13B430912) and the Scientific Research Found of Henan Provincial Department of Science and Technology (Grant no. 132300413210).
WZX and FRT carried out the experiments and drafted the manuscript. SCQ participated in the sequence alignment. XSL, WFZ and QWJ conceived the study and participated in its design. ZJW and ZGW participated in the design of the study and performed the analysis. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Liu Z, Sun Y, Yuan J, Wei H, Huang X, Han L et al (2013) High-efficiency hybrid solar cells based on polymer/PbSxSe1-x nanocrystals benefiting from vertical phase segregation. Adv Mater 25:5772–8View ArticleGoogle Scholar
- Yang X, Loos J (2007) Toward high-performance polymer solar cells: the importance of morphology control. Macromolecules 40:1353–62View ArticleGoogle Scholar
- Xin H, Kim FS, Jenekhe SA (2008) Highly efficient solar cells based on poly(3-butylthiophene) nanowires. J Am Chem Soc 130:5424–5View ArticleGoogle Scholar
- Dayal S, Reese MO, Ferguson AJ, Ginley DS, Rumbles G et al (2010) The effect of nanoparticle shape on the photocarrier dynamics and photovoltaic device performance of poly(3-hexylthiophene):CdSe nanoparticle bulk heterojunction solar cells. Adv Funct Mater 20:2629–35View ArticleGoogle Scholar
- Xie Y, Zhou W, Yin J, Hu X, Zhang L, Meng X et al (2016) Post-annealing to recover the reduced open-circuit voltage caused by solvent annealing in organic solar cells. J Mater Chem A 4:6158–66View ArticleGoogle Scholar
- Roquet S, Cravino A, Leriche P, Alévêque O, Frère P, Roncali J (2006) Hybrid systems with internal charge transfer as donor materials for heterojunction solar cells. J Am Chem Soc 128:3459–66View ArticleGoogle Scholar
- Wang T, Han L, Wei H, Zhu D, Bao X, Qiao S et al (2016) Influence of a π-bridge dependent molecular configuration on the optical and electrical characteristics of organic solar cells. J Mater Chem A 4:8784–92View ArticleGoogle Scholar
- Shi Y, Li F, Tan L, Chen Y (2013) Hybrid bulk heterojunction solar cells based on the cooperative interaction of liquid crystals within quantum dots and diblock copolymers. ACS Appl Mater Interfaces 5:11692–702View ArticleGoogle Scholar
- Chen H, Hou J, Zhang S, Liang Y, Yang G, Yang Y, Yu L, Wu Y, Li G (2009) Polymer solar cells with enhanced open-circuit voltage and efficiency. Nat Photonics 192:649–53View ArticleGoogle Scholar
- Wang JL, Wu Z, Miao JS, Liu KK, Chang ZF, Zhang RB et al (2015) Solution-processed diketopyrrolopyrrole-containing small-molecule organic solar cells with 7.0% efficiency: in-depth investigation on the effects of structure modification and solvent vapor annealing. Chem Mater 27:4338–48View ArticleGoogle Scholar
- Miao J, Chen H, Liu F, Zhao B, Hu L et al (2015) Efficiency enhancement in solution-processed organic small molecule: fullerene solar cells via solvent vapor annealing. Appl Phys Lett 106:183302View ArticleGoogle Scholar
- Xin H, Ren G, Kim FS, Jenekhe SA (2008) Bulk heterojunction solar cells from poly(3-butylthiophene)/fullerene blends: in situ self-Assembly of nanowires, morphology, charge transport, and photovoltaic properties. Chem Mater 20:6199–207View ArticleGoogle Scholar
- Nawrocki RA, Pavlica E, Celic N, Orlov D, Valant M, Mihailovic D et al (2016) Fabrication of poly(3-hexylthiophene) nanowires for high-mobility transistors. Org Electron 30:92–8View ArticleGoogle Scholar
- Chang C, Huang T, Lin Y, Lin Y, Chen C, Chu T et al (2008) Improved charge separation and transport efficiency in poly(3-hexylthiophene)–TiO2 nanorod bulk heterojunction solar cells. J Mater Chem 18:2201–7View ArticleGoogle Scholar
- Choi KC, Lee EJ, Baek YK, Lim DC, Kang YC, Kim YD et al (2015) Morphologically controlled ZnO nanostructures as electron transport materials in polymer-based organic solar cells. Electro Acta 180:435–41View ArticleGoogle Scholar
- Jeltsch KF, Schädel M, Bonekamp J, Niyamakom P, Rauscher F, Lademann HWA et al (2012) Efficiency enhanced hybrid solar cells using a blend of quantum dots and nanorods. Adv Funct Mater 22:397–404View ArticleGoogle Scholar
- Liao W, Wu J (2013) Efficient electron collection in hybrid polymer solar cells: in-situ-generated ZnO/poly(3-hexylthiophene) scaffolded by a TiO2 nanorod array. J Phys Chem Lett 4:1983–8View ArticleGoogle Scholar
- Baeten L, Conings B, Boyen H, D’Haen J, Hardy A, D’Olieslaeger M et al (2011) Towards efficient hybrid solar cells based on fully polymer infiltrated ZnO nanorod arrays. Adv Mater 23:2802–5View ArticleGoogle Scholar
- Greene LE, Law M, Yuhas BD, Yang P (2007) ZnO-TiO2 core-shell nanorod/P3HT solar cells. J Phys Chem C 111:18451–6View ArticleGoogle Scholar
- Cui Q, Liu C, Wu F, Yue W, Qiu Z, Zhang H et al (2013) Performance improvement in polymer/ZnO nanoarray hybrid solar cells by formation of ZnO/CdS-core/shell heterostructures. J Phys Chem C 117:5626–37View ArticleGoogle Scholar
- Tan F, Qu S, Wang L, Jiang Q, Zhang W, Wang Z (2014) Core/shell-shaped CdSe/PbS nanotetrapods for efficient organic–inorganic hybrid solar cells. J Mater Chem A 2:14502–10View ArticleGoogle Scholar
- Sun BQ, Marx E, Greenham NC (2003) Photovoltaic devices using blends of branched CdSe nanoparticles and conjugated polymers. Nano Lett 3:961–3View ArticleGoogle Scholar
- Tan F, Qu S, Zhang W, Wang Z (2014) Hybrid morphology dependence of CdTe:CdSe bulk-heterojunction solar cells. Nanoscale Res Lett 9:593View ArticleGoogle Scholar
- Ko WYL, Bagaria HG, Asokan S, Lina KJ, Wong MS (2010) CdSe tetrapod synthesis using cetyltrimethylammonium bromide and heat transfer fluids. J Mater Chem 20:2474–8View ArticleGoogle Scholar
- Wu P, Xin H, Kim FS, Ren G, Jenekhe SA (2009) Regioregular poly(3-pentylthiophene): synthesis, self-assembly of nanowires, high-Mobility field-effect transistors, and efficient photovoltaic cells. Macromolecules 42:8817–26View ArticleGoogle Scholar
- Cornil J, Beljonne D, Calbert JP, Bredas JL (2001) Interchain interactions in organic pi-conjugated materials: impact on electronic structure, optical response, and charge transport. Adv Mater 13:1053–67View ArticleGoogle Scholar
- Chen TA, Wu XM, Rieke RD (1995) Regiocontrolled synthesis of poly(3-alkylthiophenes) mediated by Rieke zinc: their characterization and solid-state properties. J Am Chem Soc 117:233–44View ArticleGoogle Scholar
- Nguyen LH, Hoppe H, Erb T, Günes S, Gobsch G, Sariciftci NS (2007) Effects of annealing on the nanomorphology and performance of poly(alkylthiophene):fullerene bulk-heterojunction solar cells. Adv Funct Mater 17:1071–8View ArticleGoogle Scholar
- Jung B, Kim K, Eom Y, Kim W (2015) High-pressure solvent vapor annealing with a benign solvent to rapidly enhance the performance of organic photovoltaics. ACS Appl Mater Interfaces 7:13342–9View ArticleGoogle Scholar
- Zhao L, Pang X, Adhikary R, Petrich JW, Jeffries-EL M, Lin Z (2011) Organic-inorganic nanocomposites by placing conjugated polymers in intimate contact with quantum rods. Adv Mater 23:2844–9View ArticleGoogle Scholar
- Rath AK, Bernechea M, Martinez L, Arquer FPG, Osmond J, Konstantatos G (2012) Solution-processed inorganic bulk nano-heterojunctions and their application to solar cells. Nat Photonics 6:529–34View ArticleGoogle Scholar
- Sun B, Snaith HJ, Dhoot AS, Westenhof S, Greenham NC (2005) Vertically segregated hybrid blends for photovoltaic devices with improved efficiency. J Appl Phys 97:014914View ArticleGoogle Scholar
- Murgatroyd PN (1970) Theory of space-charge-limited current enhanced by Frenkel effect. J Phys D Appl Phys 3:151–6View ArticleGoogle Scholar
- Barnea-Nehoshtan L, Kirmayer S, Edri E, Hodes G, Cahen D (2014) Surface photovoltage spectroscopy study of organo-lead perovskite solar cells. J Phys Chem Lett 5:2408–13View ArticleGoogle Scholar
- Tan F, Wang Z, Qu S, Cao D, Liu K, Jiang Q et al (2016) A CdSe thin film: a versatile buffer layer for improving performance of TiO2 nanorod array:PbS quantum dot solar cells. Nanoscale 8:10198–204View ArticleGoogle Scholar
- Zhao N, Osedach TP, Chang LY, Geyer SM, Wanger D, Binda MT et al (2010) Colloidal PbS quantum dot solar cells with high fill factor. ACS Nano 4:3743–52View ArticleGoogle Scholar